Download presentation

Presentation is loading. Please wait.

1
**Common Types of Woven Fabric**

2
**Basic weave structures**

3
Woven Structure

4
**Orientations in a Woven Fabric**

Machine direction = "warp" or "end" Perpendicular direction = "fill" or "weft" or "pick" or "woof” Frequently the warp direction corresponds with the 0°, or longitudinal direction And fill with the 90° or transverse direction However - this is not necessarily the case and should be carefully noted.

5
Woven Fabrics Generally characterized by two sets of perpendicular yarns systems One set is raised and lowered to make “sheds” (these are warp yarns) The other set is passed through these sheds, perpendicular to the warp yarns (these are fill, or pick or weft yarns)

6
Woven Fabrics The structure of the woven fabric is the pattern of interlacing between the warp and weft yarns Yarns can “float”, or not interlace for some distance within a woven fabric

7
Crimp in Weaves The crimp is defined as one less than the ratio of the yarn's actual length to the length of fabric it traverses. Crimp levels influence fiber volume fraction, thickness of fabric, and mechanical performance of fabric. High crimp leads to Reduced tensile and compressive properties Increased shear modulus in the dry fabric and the resulting composite Fewer regions for localized delamination between individual yarns.

8
Crimp Crimp is defined as the ratio of excess length of yarn in a fabric to the length of the fabric C = ly/ lf - 1 lf ly

9
Crimp Crimp is determined by the texture of the weave and the yarn size Generally, in weaving, the warp yarns have most of the crimp, the fill very little This is a direct result of the warp yarns lifting during weaving and the filling yarn being inserted along a straight path

10
Crimp Various models of crimp exist, the most rigorous developed by Pierce in the 1930s.

11
**Crimp pi = (lj – D qj) cos qj + D sin qj**

hi = (li – D qi)sin qi + D(1 - cos qi) ci = (li/pj) - 1 h1 + h2 = d1 + d2 = D Where pi =Thread spacing; li = Modular length; ci = Yarn crimp; di = Yarn diameter; hi = Modular height; qi = Weave angle D = Scale factor; sum of warp and weft diameters i,j = warp and weft directions.

12
**Crimp Simplified crimp calculations: assume triangle wave shape q**

tan q = (tf + tw) pf C= 1/cos q - 1 q tf + tw pf

13
Crimp

14
**Thickness Thickness is a difficult parameter to measure.**

Thickness is dependent on applied transverse pressure to the fabric Predictions of thickness show variation throughout the unit cell

15
Thickness

16
**Theoretical Predictions of Thickness**

Consider yarns to be ellipses with major axes ai and minor axes bi. Thickness is between 4bw + 2bf ≤ t ≤ 2bw + 2bf

17
**Theoretical Predictions of Thickness**

18
Areal Density Areal density is a measure of the weight per unit area of the fabric Usually expressed in g/m2 or oz/yd2. Areal density is a more reliable experimental metric for fabrics than thickness Areal density can be correlated to volume fraction

19
**Areal Density Areal density can be calculated as**

A = [l (1+Cw) nw Lw + w (1+Cf) nf Lf]/(w l) Where Ci = crimp of the i yarn, ni = number of i yarns per unit length, Li = linear density of the i yarn, w = width, l = length, and I=warp or weft.

20
Areal Density

21
Woven Structures 3D Woven Twill Double Cloth Satin

22
**The Effect of Yarn Crimp**

Mechanical behavior: The Effect of Yarn Crimp Plain weave Intro to composites, Hull & Clyne

23
**The Effect of Yarn Crimp**

Mechanical behavior: The Effect of Yarn Crimp Angle Interlock weave T. Norman et al. FiberTex ‘92

24
**The Effect of Yarn Crimp**

Mechanical behavior: The Effect of Yarn Crimp XYZ orthogonal weave

25
3D Weaves Layer-to-layer Through thickness XYZ

26
**Doubly Stiffened Woven Panel**

27
**Variations in Weave Design**

If large yarns are used in the warp direction and small yarns are infrequently spaced in the weft direction, the resulting fabric resembles a unidirectional material. Weaves can be formed with gradients in a single or double axis by changing yarn size across the width or length Complex shapes can be achieved through “floating” and cutting yarns to reduce total number of yarns in some section of the part

28
**Gradations through yarn size**

29
Shape through floats

30
**Issues with shaping woven fabrics**

Tailoring the cross-section of a woven fabric will generally result in a change in weave angle, a change in the distribution of longitudinal, weaver, and fill, and a change in fiber volume fraction in consequence to the change in thickness. Some fiber volume fraction effects can be controlled by tooling. The tailoring occurs in a discrete manner, using individual yarns, whereas most tooling will be approximately continuous.

31
**Example of single taper weave**

Consider a tapered panel where gradation in thickness is achieved by changing yarn size/count across the width

32
**Design of tapered woven panel**

Pick count is constant, warps and wefts per dent are modified to taper Z yarn path changes to accommodate the weave.

33
**Variation in Fiber Volume Fraction**

This variation in yarn packing results in variations in Vf for the resulting composite.

34
**Variation in weave angle**

The weave angle will also change throughout the width of the part due to varying warp yarn count and part thickness.

35
Yarn Distributions The distribution of warp, weft, and Z yarn will also vary throughout the part.

36
Variations in Modulus All mechanical properties will vary throughout the part

37
Volume Fraction Volume fraction is the percent of fiber contained within a given volume (usually the composite in question) Volume fraction can be calculated from areal density Vf = A r / t Where Vf = fiber volume fraction, A = areal density, r = density of the fibers, and t = composite thickness

38
**Process Control and Variability**

Processing Errors Damaged yarns Misplaced yarns Sources of error Machinery malfunction Machinery variability Bad control parameters Post-manufacturing deviations

39
**Distortions in Woven Fabrics**

40
**On-line Monitoring of Manufacturing**

Realtime feed-back from shedding and insertion mechanisms Visual scan of fabric surfaces Xray or neutron scan of fabric interior Using tracer yarns

41
**Three Dimensional Weaving**

Uses "standard" weaving technology Complexity of weave is limited by number of independent shedding devices Some limitations on maximum thickness of fabric due to shed size and beatup limitations

42
**Types of 3-D Woven Fabrics**

XYZ Layer-to-layer Through-thickness

43
3-D Weaving shed weaver warp filling insertion fabric movement

44
XYZ 3-D Woven Fabrics

45
**Layer-to-layer 3-D Woven Fabrics**

46
**Through thickness 3-D Woven Fabrics**

47
**Components of 3-D Woven Fabrics**

Longitudinal yarns Parallel to warp direction Weaving yarns (web yarns) Lie in warp-thickness plane Surface weavers Located at t=0, t=max Filling yarns Lie in fill-thickness plane Generally aligned with the fill direction

48
**Components of 3-D Woven Fabrics**

1/h p Fills Longitudinals Weaver t q Surface Weaver warp

49
**Physical Relationships of 3-D Woven Fabrics**

Vf = ∑ Wi / Wc Wc = (1/hp) (1/hw) t Wi = mi Ai li ll = (1/hp) lw = (1/hp)/cos(qw) ls = (1/hp)/cos(qs) lp = (1/hw)

50
**Process Variables Yarn sizes (all independent)**

Reed size (limited by yarn size) Picks per inch (limited by yarn size) Weave angle Number of filled warp positions

51
**Preform Input Parameters**

Using fiber volume (Vf), thickness (t), ply percentages (wt%) as inputs: Here r is fiber density for each n fiber type and w is the preform areal density. Yarn spacings needed for each ith system (warp, fill, weaver) can then be found using the tow linear density N:

52
**Weave Angle Projection**

1 / p p i l t a N p / p p i l t ppil tan a = N p

53
**Determining Preform Thickness Requirements**

Tows required to meet thickness can be estimated assuming a common aspect ratio (AR): b AR = a a 2 d b = = A p ab p a AR A 1 a = = d 4AR p AR - 4 2 A 3 . 9 10 in = = = a in p 6 p 6 total thickness t . 100 inches = = = = tows needed for thickness 11 tows tow thickness 2a 2 . 00455 inches

54
**3D Woven Preform Case Study**

Two sample preforms were specified, each with a 45°weave angle requested: Parameter Sample 1 Sample 2 %0° fiber 47 77 0° fiber type IM7-12k IM7-12k %90° fiber 47 17 90° fiber type IM7-12k IM7-12k %z fiber 6 6 z fiber type AS4-3k AS4-6k thickness (inches) 0.100 0.100 Volume fraction (%) 56 56 The preforms were procured from a weaver, then evaluated based on the design methodology.

55
Example Calculations Example Calculations for Sample 2, using IM7-12k graphite tows for all inputs: 6 2 Fiber direction % tows directional areal oz 10 in lb æ yd ö : ypi = 57.23 ç = density 2 è ø 1 10 .4 ypi yd 25.0 lbs 16 oz 36 in (oz/yd 2 ) 0° 77 57.23 6 æ ö 2 oz 10 in lb ç yd 90° 17 12.63 9 : ypi = 12.63 = 24 .4 ypi 2 è ø yd 25.0 lbs 16 oz 36 in ttt 6 4.46 Total 100 74.32 6 æ ö 2 oz 10 in lb ç yd z : ypi = 4.46 cos a = 7.9 ypi 2 è ø i yd 25.0 lbs 16 oz 36 in

56
**Applying the Methodology**

Sample 1 Parameter 0° 90° ttt Required Reported Required Reported Required Reported areal weight 34.9 34.9 34.9 34.9 4.5 4.5 (oz/yd 2 ) yarns per inch 67.5 67.5 67.5 67 18.2 16 Volume fraction 26.4 22.9 26.4 22.9 3.3 2.9 Sample 2 Parameter 0° 90° ttt Required Reported Required Reported Required Reported areal weight 57.2 12.5 12.6 57.2 4.5 4.5 (oz/yd 2 ) yarns per inch 110.4 24 24.4 110 8.3 6 Volume fraction 43.2 7.5 9.4 34.6 3.3 2.7

57
**Measuring the Weave Angle**

58
**Examining Volume Fraction from Input Parameters**

Evaluating Sample 2: 6 oz 10 in lb æ ç yd ö 2 6 ypi = w cos ( 22.5 ) z 2 è ø yd 11.8 lbs 16 oz 36 in w = 1 . 5 9 + 5 7 . 2 2 + 1 2 . 4 5 = 7 1 . 2 6 o z / y d 2 æ ö 2 lbs 36 in 16 oz oz ç ÷ = V .064 .100 in 71.26 f 3 è ø 2 in yd lb yd V = 5 3 . 7 % f It was calculated that 74.3 oz/yd2 was needed to meet the 56% volume fraction specified

59
**Example 6 ends per inch, 6 picks per inch, 4 picks thick**

12K AS-4 yarns long. & fill, 6K weavers, no surface weavers Weaver yarn ratio - rise/run =tan(qw) ar Thickness = 0.25 inch All warp slots filled aspect ratio = (np mp)/t

60
**Effect of Weave yarn ratio on Fiber Volume Fraction**

0.75 0.7 0.65 4 epi 6 epi 0.6 0.55 Fiber Volume Fraction 0.5 0.45 0.4 0.35 0.3 0.25 2 4 6 8 10 12 14 Weave Angle Ratio

61
**Effect of Weave Yarn Ratio on Weave Angle**

70 60 50 4 ppi Weave Angle (deg) 6 ppi 40 30 20 10 2 4 6 8 10 12 14 Weave Angle Ratio

62
**Effect of Weave Angle on Distribution**

Based on varying weave yarn ratio only 0.8 Percent longitudinal 0.7 Percent weaver Percent fill 0.6 0.5 Distribution Ratio 0.4 0.3 0.2 0.1 5 10 15 20 25 30 35 40 45 Weave Angle (deg)

63
**Effect of picks per inch on Fiber Volume Fraction**

0.45 0.4 0.35 Fiber Volume Fraction 0.3 0.25 0.2 0.15 2 4 6 8 10 12 14 16 Picks per inch

64
**Effect of picks per inch on Weave angle**

45 40 35 30 25 Weave Angle (deg) 20 15 10 5 2 4 6 8 10 12 14 16 Picks per inch

65
**Effect of Weave Angle on Distribution**

Based on varying ppi only 0.8 Percent longitudinal 0.7 Percent weaver Percent fill 0.6 0.5 Distribution Ratio 0.4 0.3 0.2 0.1 5 10 15 20 25 30 35 40 45 Weave Angle (deg)

66
**Production of Complex Shaped Weaves**

Complex shape - complex, but uniform section Very complex shape - complex, nonuniform section

67
**Production of Complex Shaped Weaves**

Consider section as consisting of rectangular pieces Develop weave parameters for each piece Develop interconnection paths

68
**Production of Very Complex Shaped Weaves**

Decompose part into rectangular and shell sections Consider impact of cutting yarns Consider "folding" type operations

69
**Ideal vs. Actual Geometry**

70
**Bad Control Parameters**

71
**Bad Control Parameters**

Bad scan of image Mistake in keying of "dots and spots" Slipped card/chain at pick insertion failure

72
**Compression Induced Errors**

73
**RTM & Handling Induced Errors**

Similar presentations

Presentation is loading. Please wait....

OK

Woven Fabric Calculations

Woven Fabric Calculations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on earthquake download Ppt on fourth and fifth state of matter summary Ppt on democracy in contemporary world class 9 Ppt on natural resources and conservation job Ppt on object-oriented programming vs procedural programming Ppt on business plan for wound care Ppt on forward contract definition Ppt on column chromatography uses Ppt on periscope Ppt on thermal power plant working